Superconductivity often emerges in the proximity of, or in competition with, symmetry-breaking ground states such as antiferromagnetism or charge density waves1,2,3,4,5 (CDW). A number of materials in the cuprate family, which includes the high transition-temperature (high-Tc) superconductors, show spin and charge density wave order5,6,7. Thus a fundamental question is to what extent do these ordered states exist for compositions close to optimal for superconductivity. Here we use high-energy X-ray diffraction to show that a CDW develops at zero field in the normal state of superconducting YBa2Cu3O6.67 (Tc = 67 K). This sample has a hole doping of 0.12 per copper and a well-ordered oxygen chain superstructure8. Below Tc, the application of a magnetic field suppresses superconductivity and enhances the CDW. Hence, the CDW and superconductivity in this typical high-Tc material are competing orders with similar energy scales, and the high-Tc superconductivity forms from a pre-existing CDW environment. Our results provide a mechanism for the formation of small Fermi surface pockets9, which explain the negative Hall and Seebeck effects10,11 and the ‘Tc plateau’12 in this material when underdoped.
Charge density waves in solids are periodic modulations of conduction electron density. They are often present in low-dimensional systems such as NbSe2 (ref. 4). Certain cuprate materials such as La2−x−yNdySrxCuO4 (Nd-LSCO) and La2−xBaxCuO4 (LBCO) also show charge modulations that suppress superconductivity near x = 1/8 (refs 6, 7). In some cases, these are believed to be unidirectional in the CuO2 plane, and have been dubbed ‘stripes’2,3. There is now a mounting body of indirect evidence that charge and/or spin density waves (static modulations) may be present at high magnetic fields in samples with high Tc: quantum oscillation experiments on underdoped YBa2Cu3Oy (YBCO) have revealed the existence of at least one small Fermi surface pocket9,10, which may be created by a charge modulation11. More recently, nuclear magnetic resonance (NMR) studies have shown a magnetic-field-induced splitting of the Cu2F lines of YBCO (ref. 13). An important issue is the extent to which the tendency towards charge order exists in high-Tc superconductors2,3.
Here we report a hard (100 keV) X-ray diffraction study, in magnetic fields up to 17 T, of a detwinned single crystal of YBa2Cu3O6.67 (with ortho-VIII oxygen ordering8,12, Tc = 67 K and p = 0.12, where p is the hole concentration per planar Cu). We find that a CDW forms in the normal state below TCDW≈135 K. The charge modulation has two fundamental wave vectors qCDW = q1 = (δ1,0,0.5) and q2 = (0,δ2,0.5), where δ1≈0.3045(2) and δ2≈0.3146(7), with no significant field- or temperature-dependence of these values. The CDW gives rise to satellites of the parent crystal Bragg peaks at positions such as Q = (2±δ1,0,0.5). Although the satellite intensities have a strong temperature and magnetic field dependence, the CDW is not field-induced and is unaffected by field in the normal state. Below Tc it competes with superconductivity, and a decrease of the CDW amplitude in zero field becomes an increase when superconductivity is suppressed by field. A very recent paper14 reports complementary resonant soft X-ray scattering experiments performed on (Y,Nd)Ba2Cu3O6+x as a function of doping and in the absence of a magnetic field. The results are broadly in agreement with our zero field data.
Figure 1a,g shows scans through the (2−δ1,0,0.5) and (0,2−δ2,0.5) positions at T = 2 K. Related peaks were observed at (2+δ1,0,0.5) and (4−δ1,0,0.5) (see Supplementary Fig. S3). The incommensurate peaks are not detected above 150 K (Fig. 1c). From the peak width we estimate that the modulation has an in-plane correlation length ξa≈95±5 Å (at 2 K and 17 T—see Methods). The existence of four similar in-plane modulations (±δ1,0) and (0,±δ2) indicates that the modulation is associated with the (nearly square) CuO2 planes rather than the CuO chains. The present experiment cannot distinguish between 1−q and 2−q structures, that is, we cannot tell directly whether modulations along the a and b directions co-exist in space or occur in different domains of the crystal. However, Bragg peaks from the two CDW components have similar intensities and widths (Fig. 1b,g) despite the orthorhombic crystal structure, which breaks the symmetry between them. This suggests that q1 and q2 are coupled, leading to the co-existence of multiple wave vectors, as seen in other CDW systems such as NbSe2 (ref. 4). The scan along the c* direction in Fig. 1d has broad peaks close to l = ±0.5 reciprocal lattice units (r.l.u.), indicating that the CDW is weakly correlated along the c direction, with a correlation length ξc of approximately 0.6 lattice units.
In zero field, the intensity of the CDW Bragg peak (Fig. 2) grows on cooling to Tc, below which it is partially suppressed. For T>Tc, a magnetic field applied along the c direction has no effect. Below Tc it causes an increase of the intensity of the CDW signal (Figs 1a and 2). At T = 2 K, the intensity grows with applied magnetic field (Fig. 2b) and shows no signs of saturation up to 17 T. The magnetic field also makes the CDW more long-range ordered (Fig. 2c). In zero magnetic field, the q-width varies little with temperature. However, below Tc in a field, the CDW order not only becomes stronger, but also becomes more coherent, down to a temperature Tcusp below which the intensity starts to decrease (Figs 2 and 4). All of this is clear evidence for competition between CDW and superconducting orders.
Non-resonant X-ray diffraction is sensitive to modulations of charge density and magnetic moments. In our case, the expected magnetic cross-section is several orders of magnitude smaller than our observed signal, which must therefore be due to charge scattering. NMR measurements on a sample of the same composition as ours13 indicate that the CDW is not accompanied by magnetic order, and this is confirmed by soft X-ray measurements, which would also be sensitive to fluctuating order14. Charge density modulations in solids will always involve both a modulation of the electronic charge and a periodic displacement of the atomic positions15. We are more sensitive to the atomic displacements than to the charge modulation because ions with large numbers of electrons (as in YBCO) dominate the scattering (see Supplementary Information).
NMR data13 suggest that CDW order only appears below T≈67 K and H>9 T, whereas with X-rays we observe CDW order in zero field up to 135 K. This apparent discrepancy may arise from differing timescales of various probes (see Supplementary Information for further discussion). X-ray diffraction experiments are usually interpreted as measuring the static order of a given structure, but, if performed with wide energy acceptance, are also sensitive to short-lived structures. Thus, it is possible that the observed CDW is quasi-static and only frozen on the NMR timescale (≈3 ns) at high fields and lower temperatures.
The intensities of the incommensurate Bragg peaks are sensitive to atomic displacements parallel to the total scattering vector Q. The comparatively small contribution to Q along the c* direction from l = 0.5 r.l.u. means that our signal for a (h, 0, 0.5) peak is dominated by displacements parallel to the a direction. (There will also be displacements parallel to the c direction but we are essentially insensitive to them in our present scattering geometry). Our data indicate that the incommensurate peaks are much stronger if they are satellites of strong Bragg peaks of the form at positions such as . This indicates that the satellites are caused by a modulation of the parent crystal structure. The fact that the scattering is peaked at l = ±0.5 r.l.u. means that neighbouring bilayers are modulated in antiphase. The two simplest structures (Fig. 3a,b) compatible with our data (see Supplementary Information) involve the neighbouring CuO2 planes in the bilayer being displaced in the same (bilayer-centred) or opposite (chain-centred) directions, resulting in the maximum amplitude of the modulation being on the CuO2 planes or CuO chains respectively. In their 2−q form, these structures would lead to the in-plane ‘checkerboard’ pattern shown in Fig. 3c. Scanning tunnelling microscopy studies of other underdoped cuprates16 and of field-induced CDW correlations in vortex cores17 also support the tendency towards checkerboard formation18, although disorder can cause small stripe domains to mimic checkerboard order19. Our observation of a CDW may be related to phonon anomalies20, which suggest that in YBCO near p≈1/8 there are anomalies in the underlying charge susceptibility for q≈(0,0.3).
Cuprate superconductors show strong spin correlations, and the interplay between spin and charge correlations may be at the heart of the high-Tc phenomenon. The spin correlations are largely dynamic, with energies up to several hundred meV. YBa2Cu3O6+x and La2−x(Ba,Sr)xCuO4+δ show incommensurate magnetic order, which can be enhanced by suppressing superconductivity with an applied magnetic field21,22,23,24; this has some analogies with the CDW order observed here. The magnetic order is static on the ∼ 1 meV frequency scale of neutron diffraction and has been detected in lightly doped YBa2Cu3O6+x for p≤0.082(ref. 21), and moderately doped La2−xSrxCuO4 for p≤0.14 (ref. 24). The YBa2Cu3O6.67 (p≈1/8) sample studied here is expected to have a relatively large spin gap, ℏω≈20 meV (ref. 25), in its magnetic excitations at low temperature, making it unlikely that it orders magnetically. As discussed earlier, this is confirmed by other measurements13,14, so the CDW does not seem to be accompanied by spin order. Moreover, there is no obvious relationship between qCDW and the wave vector of the incipient spin fluctuations qSF≈(0.1,0) of similarly doped samples25.
It is interesting to note that TCDW corresponds approximately with TH (Fig. 4), the temperature at which Hall effect measurements suggest that Fermi surface reconstruction begins26. A CDW that breaks translational symmetry provides a natural mechanism for Fermi surface reconstruction and the formation of pockets. From the negative Hall and Seebeck coefficients10,11,26, it was inferred that the Fermi pocket observed by quantum oscillations9 is electron-like10. The exact structure of the low-temperature reconstructed Fermi surface is still debated, although recent high-field specific heat experiments place constraints on the possibilities and suggest a small number of pockets27 (see Supplementary Information). It is interesting to compare the LDA Fermi surface of YBCO (ref. 28) with qCDW (Fig. 3d and Supplementary Information). The electronic states most obviously connected by qCDW are the bonding bands at and near the zone boundary, which lie near the anti-nodal region of the superconducting gap, where the pseudogap is also maximized.
Our results have important implications for the phenomenology and phase diagram of the cuprates (Fig. 4). A simple Landau theory (see Supplementary Information) shows that Tc will be suppressed below the value it would have in the absence of the CDW. We speculate that this is reflected in the shape of the superconducting dome12 (Fig. 4). One of the defining properties of underdoped cuprates such as ortho-VIII YBCO is the pseudogap. This develops at the ‘crossover’ temperature T* (for YBa2Cu3O6.67, T*≈220 K), where there is a suppression of low-energy electronic states, evidence for ‘Q = 0’ magnetic order29 and rotational anisotropy appears in various physical properties, such as the Nernst effect30. The CDW reported here develops at TCDW≈135 K, inside the pseudogap state. From Fig. 2a,c we can identify the temperature Tcusp(H) where the suppression of the CDW begins. The level of this competition indicates that the CDW and superconductivity have similar energy scales (10–30 meV), unlike NbSe2 where the CDW order is not significantly suppressed by superconductivity4. Tcusp(H) (Fig. 4) seems to correspond to the temperature Tn(H) at which superconductivity in the mixed state can be identified from transport measurements rather than the appearance of zero resistance.
We draw attention to the situation in the cuprates that many different kinds of order, such as superconductivity, pseudogap, CDW and antiferromagnetism, occur on comparable temperature scales. When they compete, they do so on an almost equal footing. We may suspect that this is not accidental, and that these various orders are ‘intertwined’31. In this context, we can view our present results as indicating that the electron system has a tendency towards two ground states: a charge density wave, which breaks translational symmetry and involves electron–hole correlations, versus superconductivity, which breaks gauge symmetry and involves electron–electron correlations. We note that the q-vectors of the CDW lie close to the separation of pieces of Fermi surface that have maximum superconducting gap at optimal doping and have the same sign of the order parameter.
Our experiments used 100 keV hard X-ray synchrotron radiation from the DORIS-III storage ring at DESY, Hamburg, Germany. We installed a recently developed 17 T horizontal cryomagnet designed for beamline use on the triple-axis diffractometer at beamline BW5. The sample was mounted by gluing it over a hole in a temperature-controlled aluminium plate within the cryomagnet vacuum and was thermally shielded by thin Al and aluminized mylar foils glued to this plate. The sample temperature could be controlled over the range ∼ 2–300 K. The incoming and outgoing beams passed through 1 mm thick aluminium cryostat vacuum windows, which gave a maximum of ∼±10° input and output angles relative to the field direction, which was parallel to the sample c axis within <1°. Between the beam access windows and the sample plate, there were further aluminium foil thermal radiation shields at liquid nitrogen temperature. A 2 mm square aperture collimated the incoming beam, so that it passed mainly through the part of the sample over the hole in the aluminium plate, greatly reducing background scattering by the plate. Further slits before the analyser and the detector removed scattering by the cryostat windows and nitrogen shields. The scattering plane (a*–c*) was horizontal. The cryomagnet was mounted on a rotation stage with a goniometer giving χ tilt about the field axis. The sample was initially mounted with its a axis nearly horizontal. The χ goniometer allowed the exact alignment of this axis using the (2 0 0) Bragg peak and could also be used for low-resolution scans in the b* direction. Magnetic fields were applied with the sample heated above Tc; it was then field-cooled to base temperature. When fields were applied, minor changes in the position and angle of the sample holder were observed; these were corrected by use of horizontal and vertical motion stages under the cryostat rotation stage, and by realigning on the (2 0 0) Bragg peak. During temperature scans, realignment on the (2 0 0) Bragg peak was performed automatically at every temperature point to ensure that all measurements were centred. After results had been obtained with the a axis horizontal, the sample was remounted with the b axis horizontal for further measurements. The YBa2Cu3O6.67 sample had dimensions a×b×c = 3.1×1.7×0.6 mm3 and mass 18 mg. The superconducting transition temperature Tc = 67 K (width: 10%–90% = 1.1 K) was derived from a zero-field-cooled magnetization curve at 0.1 mT. The single crystal was 99% detwinned and the Cu–O chains were ordered with the ortho-VIII structure by standard procedures12.
The diffracted intensities from the CDW, shown in Fig. 1, are composed of an incommensurate lattice modulation peak on a smoothly varying background. The background along (h, 0, 0.5) mainly originates from the tails of the ortho-VIII peaks (see Supplementary Information). It varies strongly from one Brillouin zone to another; for example, the background around (2.7, 0, 0.5) is an order of magnitude larger than around (1.7, 0, 0.5). The background has essentially no field dependence (Fig. 1a–c) so subtracting the zero-field from high-field data is a simple way to eliminate the background. This reveals the field-enhanced signal inside the superconducting state (Fig. 1a–d).
As there is a weak temperature dependence in the background (Fig. 1a–c), it is not possible to eliminate it by subtracting a high-temperature curve. Therefore, to obtain the temperature dependences shown in Fig. 2, we fitted the data to a Gaussian function G(Q) and modelled the background by a second-order polynomial B(Q) = c0+c1Q+c2Q2. The constants c0, c1 and c2 have a small but significant temperature dependence. The low counting statistics resulted in Gaussians fitting equally well as other possible lineshapes such as Lorentzians.
The signal-to-background ratio is best for the (2−δ1, 0, 0.5) peak due the weaker structural ortho-VIII peak (see Supplementary Fig. S2). From the Gaussian fits to the (2−δ1, 0, 0.5) satellite peak at 2 K and 17 T we can estimate the correlation length ξ along the three crystal axis directions. We define ξ = 1/σ, where σ = (σmeas2−σR2)0.5 is the measured Gaussian standard deviation corrected for the instrument resolution σR and expressed in Å−1. Along the a axis direction, we find σ = 6.4×10−3 r.l.u.≡1.1×10−2 Å−1, and hence ξa = 95±5 Å. Deconvolving the poor instrumental resolution along the b axis direction for the (2−δ1, 0, 0.5) peak yields a similar correlation length ξb∼ξa.
Mathur, N. D. et al. Magnetically mediated superconductivity in heavy fermion compounds. Nature 394, 39–43 (1998).
Kivelson, S. A. et al. How to detect fluctuating stripes in the high-temperature superconductors. Rev. Mod. Phys. 75, 1201–1241 (2003).
Vojta, M. Lattice symmetry breaking in cuprate superconductors: Stripes, nematics, and superconductivity. Adv. Phys. 58, 699–820 (2009).
Moncton, D. E., Axe, J. D. & DiSalvo, F. J. Neutron scattering study of the charge–density wave transitions in 2H–TaSe2 and 2H–NbSe2 . Phys. Rev. B 16, 801–819 (1977).
Demler, E., Sachdev, S. & Zhang, Y. Spin-ordering quantum transitions of superconductors in a magnetic field. Phys. Rev. Lett. 87, 067202 (2001).
Tranquada, J. M. et al. Evidence for stripe correlations of spins and holes in copper oxide superconductors. Nature 375, 561–563 (1995).
Fujita, M., Goka, H., Yamada, K., Tranquada, J. M. & Regnault, L. P. Stripe order, depinning, and fluctuations in La1.875Ba0.125CuO4 and La1.875Ba0.075Sr0.05CuO4 . Phys. Rev. B 70, 104517 (2004).
Von Zimmermann, M. et al. Oxygen-ordering superstructures in underdoped YBa2Cu3O6+x studied by hard x-ray diffraction. Phys. Rev. B 68, 104515 (2003).
Doiron-Leyraud, N. et al. Quantum oscillations and the Fermi surface in an underdoped high-T c superconductor. Nature 447, 565–568 (2007).
LeBoeuf, D. et al. Electron pockets in the Fermi surface of hole-doped high-T c superconductors. Nature 450, 533–536 (2007).
Laliberté, F. et al. Fermi-surface reconstruction by stripe order in cuprate superconductors. Nature Commun. 2, 432 (2011).
Liang, R. et al. Evaluation of CuO2 plane hole doping in YBa2Cu3O6+x single crystals. Phys. Rev. B 73, 180505 (2006).
Wu, T. et al. Magnetic-field-induced charge-stripe order in the high-temperature superconductor YBa2Cu3Oy . Nature 477, 191–194 (2011).
Ghiringhelli, G. et al. Long-range incommensurate charge fluctuations in (Y,Nd)Ba2Cu3O6+x . Science 337, 821–825 (2012).
Abbamonte, P. Charge modulations versus strain waves in resonant x-ray scattering. Phys. Rev. B 74, 195113 (2006).
Schmidt, A. R. et al. Electronic structure of the cuprate superconducting and pseudogap phases from spectroscopic imaging. New J. Phys. 13, 065014 (2011).
Hoffman, J. E. et al. A four unit cell periodic pattern of quasi-particle states surrounding vortex cores in Bi2Sr2CaCu2O8+δ . Science 295, 466–469 (2002).
Wise, W. D. et al. Charge-density-wave origin of cuprate checkerboard visualized by scanning tunnelling microscopy. Nature Phys. 4, 696–699 (2008).
Robertson, J. A. et al. Distinguishing patterns of charge order: Stripes or checkerboards. Phys. Rev. B 74, 134507 (2006).
Reznik, D. et al. Electron-phonon coupling reflecting dynamic charge inhomogeneity in copper oxide superconductors. Nature 440, 1170–1173 (2006).
Haug, D. et al. Neutron scattering study of the magnetic phase diagram of underdoped YBa2Cu3O6+x . New J. Phys. 12, 105006 (2010).
Lake, B. et al. Antiferromagnetic order induced by an applied magnetic field in a high-temperature superconductor. Nature 415, 299–302 (2002).
Khaykovich, B. et al. Enhancement of long-range magnetic order by magnetic field in superconducting La2CuO4+y . Phys. Rev. B 66, 014528 (2002).
Chang, J. et al. Tuning competing orders in La2−xSrxCuO4 cuprate superconductors by the application of an external magnetic field. Phys. Rev. B 78, 104525 (2008).
Dai, P., Mook, H. A., Hunt, R. D. & Dogan, F. Evolution of the resonance and incommensurate spin fluctuations in superconducting YBa2Cu3O6+x . Phys. Rev. B 63, 054525 (2001).
LeBoeuf, D. et al. Lifshitz critical point in the cuprate superconductor YBa2Cu3Oy from high-field Hall effect measurements. Phys. Rev. B 83, 054506 (2011).
Riggs, S. C. et al. Heat capacity through the magnetic-field-induced resistive transition in an underdoped high-temperature superconductor. Nature Phys. 7, 332–335 (2011).
Carrington, A. & Yelland, E. A. Band-structure calculations of Fermi-surface pockets in ortho-II YBa2Cu3O6.5 . Phys. Rev. B 76, 140508 (2007).
Li, Y. et al. Unusual magnetic order in the pseudogap region of the superconductor HgBa2CuO4+δ . Nature 455, 372–375 (2008).
Daou, R. et al. Broken rotational symmetry in the pseudogap phase of a high-T c superconductor. Nature 463, 519–522 (2010).
Berg, E., Fradkin, E., Kivelson, S. A. & Tranquada, J. M. Striped superconductors: How spin, charge and superconducting orders intertwine in the cuprates. New J. Phys. 11, 115004 (2009).
Achkar, A. J. et al. Distinct charge orders in the planes and chains of ortho-III ordered YBa2Cu3O6+δ identified by resonant elastic x-ray scattering. Preprint at http://arxiv.org/abs/1207.3667.
Chang, J. et al. Nernst effect in the cuprate superconductor YBa2Cu3Oy: Broken rotational and translational symmetries. Phys. Rev. B 84, 014507 (2011).
We thank B. L. Gyorffy, M. W. Long, J. A. Wilson, A. J. Schofield, J. R. Cooper, J. W. Loram, S. A. Kivelson, L. Taillefer, C. Bourbonnais, C. Proust and A. Kapitulnik for discussions and R. Nowak, G. R. Walsh and J. Blume for technical assistance. This work was supported by the EPSRC (grant numbers EP/G027161/1 and EP/J015423/1), the Wolfson Foundation, the Royal Society, the Danish Agency for Science, Technology and Innovation under DANSCATT and the Swiss National Science Foundation through NCCR-MaNEP and grant number PZ00P2_142434. J.C., N.B.C. and J.M. are grateful to L. Braicovich, G. Ghiringhelli, B. Keimer and M. Le Tacon for communicating their results to them after this experiment was completed.
The authors declare no competing financial interests.
About this article
Cite this article
Chang, J., Blackburn, E., Holmes, A. et al. Direct observation of competition between superconductivity and charge density wave order in YBa2Cu3O6.67. Nature Phys 8, 871–876 (2012). https://doi.org/10.1038/nphys2456
This article is cited by
Unconventional charge order and superconductivity in kagome-lattice systems as seen by muon-spin rotation
npj Quantum Materials (2023)
Nature Communications (2023)
Nature Communications (2023)
Nature Communications (2023)
npj Quantum Materials (2023)